Ames Laboratory Technical Reports
A proposed model for high temperature creep of
Robert E. UhrigIowa State University
Follow this and additional works at:
Part of the
Chemical Engineering Commons
, and the
This Report is brought to you for free and open access by the Ames Laboratory at Iowa State University Digital Repository. It has been accepted for inclusion in Ames Laboratory Technical Reports by an authorized administrator of Iowa State University Digital Repository. For more information, please email@example.com.
Uhrig, Robert E., "A proposed model for high temperature creep of tantalum" (1960).Ames Laboratory Technical Reports. 21.
A proposed model for high temperature creep of tantalum
A model for the creep of tantalum at elevated temperature has been presented in which the increase in strain rate with strain is related to the reduction of .the cross-sectional area accompanying strain. Comparison of experimental data with the proposed theory indicates that the dominant creep mechanism beyond the second stage of creep starts at a point of highest temperature or at a stress concentration, spreads throughout the volume in the immediate vicinity, and eventually results in localized "necking down."
Chemical Engineering | Chemistry
Chemistry-Gener al (UC ··4) TID 4500, August 1, 1959
UNITED STATES. ATOMIC ENERGY COMMISSION
Research and Development Report
A PROPOSED MODEL FOR HIGH
TEMPERATURE CREEP OF TANTALUM
Robert E. Uhrig
May 196 0
Ames Laboratory at
Iowa State University of Science and Technology F. H. Spedding, Director
Contract W -7405 eng-82
This report is distributed according to the category Chemistry-General (UC-4) as listed in TID-4500 , August 1 , 1959.
This report was prepared as an account of Government sponsored work. Neither the United States , nor the Commission, nor any person acting on behalf of the Commission:
A. Makes any warranty of representation, express or implied, with respect to the accuracy, completeness, or usefulness of
the information contained in this report, or that the use of
any information, apparatus, method, or process disclosed in this report may not infringe privately owned rights; or
B. Assumes any liabilities with respect to the use of, or for damages resulting from the use of any information, apparatus, me'thod, or process disclosed in this report.
As used . in the above, ''person acting on behalf of the Commission" includes any employe·e or contractor of the Commission, or employee of such
contractor, to the extent that such employee or contractor of the Commis -sian, or employee of such contractor,prepares, disseminates, or provides access to, 'any informati onwursuant to ' his employment or contract with the Commission, or his employment with S\l,hh contractor.
Printed in USA. Price
$0. 75 Available from the
ABSTRACT . . . .
ANALYSIS . . . .
CONCLUSIONS . . . .
A PROPOSED MODEL FOR HIGH TEMPERATURE CREEP OF TANTALUM
Robert E . Uhrig
Abstract - -A model for the creep of tantalum at elevated
temperature has been presented i n which the increase in strain
rate with strain is related to the reduction of .the cross-sectional
area accompanying strain. Comparis on of exper i mental data
with the proposed theory indicates that the dominant creep
mechanis m beyond t he second stage of creep starts at a po i nt
of highe s t temperatu r e or at a , stress concentration, spreads
throughout the volume in the i mmediate vicinity , and eventually
res ults in localized "necking down . "
Observations on creep of tantalum at 800.,.C by Murphy and Uhr i g 1 i
n-d icate that the creep curve (strain vs tim~) can be separated into four
stages: the i nitial stage in which strain hardening occurs and the strain
(1) G. Mur phy and R. E . Uhrig, U. S. Atomic Energy Report IS - 26,
rate decreases, the secondary stage in which the strain rate remains
con-. stant, the exponential stage in which strain and strain rate both i ncrease
exponentially, .and the final stage in which the creep r ate increases with
time at a rate greater than in the exponential stage . Since the strain and
strain rate both vary exponentially with -time during the exponential
stage of creep, the strain rate is proportional to the strain. This
indi-cates that the strain rate is influenced by the amount of strain in the
ma-terial and that high temperature creep may involve progressive damage.
One form of change which continually takes place during straining is
the reduction of the cross-sectional area of the specimen as it elongates .
As most creep machines are constant load rather than constant stress
devices, the stress increases as the cross-sectional area decreases.
For purposes of analysis the reduction of area is generally assumed to
be uniform throughout the gage length of the specimen. However, a
considerable amount of "necking down" ia a relative small portion of
the specimen does occur immediately prior to failure. In examining
several specimens for which the test was. discontinued when it became
evident that failure was eminent, the usual necked down region was
found. However, the diameter of the specimen along the rest of the
specimen was relatively constant, usually 0. 004 or 0. 00~ in. less
Let us consider the b e havi or of a specimen undergoing a creep test.
The specimen has been machined to a tol erance of+ 0. 001 in. in diameter
and then polished to a fine finish . The furnace controls have been adjusted
to give as uniform a temperature distribution as possible along the gage
length. Generous fillets at the end of the gage length have been used to
eliminate stress concentrations. However, somewhere along the specimen
there is one spot which is hotter than any other spot, or there is one point
at which the stress is greater due to the inclusion of an impurity or a
machining scratch which causes a: stress concentration. Since the creep
&is quite sensitive to both stress CT'"and temperature T as
indicated in the
rela~ionship gi~enby Dorn2
- - -dt K'
where K' is a structure sensitive parameter, AH is the activation energy
for creep and R is the gas constant. If the strain takes place in the
vicinity of the point where the stress or temperature is a maximum,
the cross-sectional area will be· reduced locally. This causes the
stress to increase at this point and in turn increase the localized strain
and strain rate . In the abse~ce of some sort of strain-hardening (or
(2) Dorn, J. E . , "Modern Chemistry for the Engineer and Scientist ,",~,
276 (G. Ross Robertson, ed., McGraw-Hill Book Company, New
stress-relieving) mechanism, the specimen would fail almost immediately
at this point. If an effective strain-hardening mechanism Were present,
the strength of the material at this point would increase, causing the
localized straining to cease and probably start elsewhere. If a partially
effective strain-hardening mechanism were present,
it is possible that
the strain could be confined to a local area without causing immediate
failure, The existence of such a partially effective strain-hardening
mechanism at the high temperature (800°C} under consideration is
postu-lated for the analysis which follows.
Another factor which contributes to the increasing strain rate is
the use of nominal (engineering) strain
€rather than true stliain
Since the original gage length is less than the actual gage length at any
time during the test, the use of engineering strain gives strains and
strain rates which are higher than 1thk corresponding true strains and
strain rates. True strain
£.can be shown to be
=ln ( 1
E: · ) .
The derivative of Eq. (2) gives the true strain rate
dE. = 1
dt 1 +€ dt
which is less than nominal strain rate by a factor (1
stress is defined as
the gage length
o<.in which deformation occurs changed as the t es t
pro-gressed. In order t o determine the variation of CX: w ith strain, plots
of strain vs strain rate w e r e dr awn for se v eral v a lu es of
a<.The con-stant K for each ol..was calculated using as a boundary condition the
values of strain and strain rate obtained when the expone ntial stage of
creep is extrapolated back to time t
The plots of strain rate ~ strain for six values of
o/.are shown in
Figs. 3 and 4 for the two tests. Experimental data from the two tests
are superimposed on the families of calculated curves. The inter
sec-tion o:f the experimental and calculated curves gives the fracsec-tion
gage l e ngth in which strain occurs as the strain in c reases. Fig. 5 shows
that the fraction
of...increases as the strain increases.
If it is postulated that the exponential stage of creep extends back
to time t
=o and that the first and second stages of creep are
respec-tively transient and constant in nature, then it would appear that the
initial plastic action of the exponential creep phenomenon takes place
in a very small volume. As the strain increases, the portion of the
specimen in which plastic action tak es place continues to increase in
an almost linear manner as indicated in Fig. 5. This increase in the
volume participating in creep during the exponential stage gives
point where the temperature is the highest or the stress is the greatest .
The partially effective strain-hardening mechanism postulated in this
theory then causes the straining to spread throughout the volume in
the immedi ate v i cini ty and eventually re sults in localized "necking down".
A model for the creep of tantalum at elevated temperatures is
pre-sented. The increase in strain rate with strain is related to the increase
i n stress caused by the reduction in cross-sectional area accompanying
atrain. Since it is believed that creep beyond the second stage is
con-fined to a local area , it was as sumed in the model that only a small
fract i on of the gage length actively participated in the yielding . The
presence of a partially effective strain-hardening mechanism is also
Comparison of the experimental d ata with the proposed theory
indi-cated that the participating fraction of the gage length increased as the
strain increased. It is concluded that the dominant creep mechanism
beyond the second stage of creep actually starts at a point .of highest
tempe rature o r at a stress c o ncentration , spreads throughout the
v olume in the i mmediate vicinity, and eventually results in localized